J. Mater. Environ. Sci. 5 (4) (2014) 975-982 ISSN : 2028-2508 CODEN: JMESCN

Ainane et al.

Removal of hexavalent chromium from aqueous solution by raw and chemically modified seaweed Bifurcaria bifurcata T. Ainane1,2, A. Abourriche1 , M. Kabbaj2, M. Elkouali2, A. Bennamara1, M. Charrouf1, M. Talbi2 (1) Biomolecules and organic synthesis laboratory, Faculty of Sciences Ben Msik, University Hassan II, BP 7955 casablanca 20660, Morocco. (2) Laboratory of Analytical Chemistry and Physical Chemistry of Materials, Faculty of Sciences Ben Msik, University Hassan II, BP 7955 casablanca 20660, Morocco. Received 11 Nov 2013, Revised 8 May 2014, Accepted 8 May 2014. Email: [email protected] Tel :00 212 (0) 6 60 39 30 90

Abstract The presence of hexavalent chromium Cr(VI) in wastewater is a potential hazard to aquatic animals and humans. There are various mechanisms proposed, kinetic models used and adsorption isotherms employed for the efficient removal of hexavalent chromium from industrial and municipal wastewaters using biosorbents. Biosorption of heavy metals is a most promising technology involved in the removal of toxic metals from industrial waste streams and natural waters. Metal removal treatment systems using natural materialsare cheap because of the low cost of sorbent materials used and may represent a practical replacement to conventional processes. The objective of this study is to assess the uptake of hexavalent chromium from aqueous solutions onto Bifurcaria bifurcata algae raw and chemically modified. The biosorption data of hexavalent chromium by marine brown algae Bifurcaria bifurcata, which was raw RB and chemically modified by hydrochloric acid AB, has been used for kinetic studies based on fractional power, Elovich, pseudo-first order, pseudosecond order and intraparticle diffusion rate expressions. four two parameter biosorption isotherm models, Freundlich, Langmuir, Dubinin – Radushkevich, Temkin are tested for their applicability. The time-dependent Cr(VI) biosorption data were well-described by fractional power and Elovich kinetic model. Among the two-parameter models, the Langmuir model produces the best fit. Comparing our results with other previous work on the brown algae, shows the value of materials developed from Bifurcaria bifurcata and allows us to offer them as adsorbent materials. Keywords: Hexavalent chromium, Bifurcaria bifurcata, Biosorption, Kinetics, Equilibrium models.

1. Introduction The presence of toxic heavy metals in water resulting from rapid industrialization and technological advances is a worldwide environmental problem [1-4]. One of the heavy metals that has been a major focus in water and wastewater treatment is chromium and the hexavalent form of it has been considered to be more hazardous due to its carcinogenic properties [5-7]. Chromium has been considered as one of the top 16th. Toxic pollutants and because of its carcinogenic and teratogenic characteristics on the public, it has become a serious health concern [8]. Chromium can be released to the environment through a large number of industrial operations, including metal finishing industry, iron and steel industries and inorganic chemicals production [9]. Extensive use of chromium results in large quantities of chromium containing effluents which need an exigent treatment. The permissible limit of chromium for drinking water is 0.1 mg/L (as total chromium) in EPA standard (United States Environmental Protection Agency). In addition, World Health Organization standard for Cr(VI) concentration in drinking water is 0.05 mg/L [10-11]. Removal of heavy metals from aqueous effluents has conventionally been accomplished through a range of abiotic processes [12-14]. However, these processes can be expensive and not fully effective. Recently, increasing interest in the application of materials of biological origin in heavy metals removal from diluted, large volume solutions has been observed. Sorption with bio-materials has become an alternative to traditional methods of industrial wastewaters treatment, such as precipitation, adsorption, coagulation, … [15-17] and it is relatively inexpensive, non-hazardous, and may permit recovery of the metals from the sorbing biomass [18]. The potential 975

J. Mater. Environ. Sci. 5 (4) (2014) 975-982 ISSN : 2028-2508 CODEN: JMESCN

Ainane et al.

of nonviable brown seaweeds in the recovery of heavy metal ions from aqueous effluents has been well demonstrated [19,20]. The objective of this study was to evaluate the adsorption capacity of chromium on substrates obtained from the brown seaweed Bifurcaria bifurcata. The choice of the latter is mainly based on purely economic considerations, because we are always looking for natural materials with no obvious utility in order to exploit them for very specific tasks, either in its raw state or after certain operations do not require large investments in energy supply or material. The main objective is to enhance this marine natural resource and use for water-pollution control and preservation of ecological balance.

2. Materials and methods 2.1 Biomass and chemical modification The brown alga Bifurcaria bifurcata was collected from the Dar Bouaaza beach (Casablanca), Morocco in December 2009. The alga was washed with running water and with deionized water. The washed biomass was oven-dried at 60 ◦C for 24 h, crushed with an analytical mill, sieved (size fraction of 0.50 mm). The resulting dried biomass was designated as the raw biomass (RB) in the present study. A 100 g raw biomass was activated in 1M solution of hydrochloric acid at 25 °C for 2h and the mixture was separated by centrifugation and washed thoroughly with distilled water. It was dried in an oven at 60 °C for 24 h. resulting dried biomass was designated as the actived biomass (AB). 2.2 Sorption experiments and analytical method All the experiments were conducted at a constant temperature of 25±1 °C and at a constant pH = 5.8 to be representative of environmentally relevant conditions. Batch kinetics and equilibrium sorption experiments were carried out in 250mL Erlenmeyer flasks containing Potassium dichromate solutions (100 mL) of known concentrations, which varied from 30 to 50 mg L−1. Known amounts of biomass were added to each flask and the mixtures were agitated on the rotary shaker. After the sorption was reached, The change in Cr(VI) concentration due to sorption was determined colorimetrically (Shimadzu 1240 spectrophotometer) according to Standard Methods [21]. A purple-violet colored complex was developed in the reaction between Cr(VI) and 1,5-diphenylcarbazide in acidic condition. Absorbance was measured at wavelength (λ) 540 nm. 2.3 Chromium uptake capacities The amount of Cr(VI) sorbed at equilibrium, q (mg.g−1), which represents the metal uptake, was calculated from the difference in metal concentration in the aqueous phase before and after adsorption, according to the following equation [22] : (C0 -Ce ) q= m C0 and Ce are the initial and equilibrium concentration of Cr(VI) in solution (mg.l−1), respectively, and m is the mass of dry seaweed (g). where V is the volume of Cr(VI) solution (L). Fractional power [23], Elovich [24], pseudo-first order [25], pseudo-second order [24] and intraparticle diffusion [26] rate equations have been used for modeling the kinetics of Cr(VI) sorption (Table 1). Table 1: Kinetic biosorption models. Model Fractional power Elovich pseudo-first order pseudo-second order

Equation qt = kp .tν

1 .Ln(αE .βE .t) βE qt = qe,1P (1-e-k1p .t ) qt =

qt =

k2p .q2e,2P .t

linear expression Ln qt = ν.Ln t + Ln kp Ln(αE .βE ) 1 qt = + .Lnt βE βE Ln qe -qt = -k1p .t + Ln qe,1P 1 1 1 = + qt k2p .qe,2P .t qe,2P

1 + k2p .qe,2P .t Intraparticle diffusion qt = kD .t1/2 + CD To examine the relationship between sorbed and aqueous concentration at equilibrium, various two-parameter sorption isotherm models like Freundlich [27], Langmuir [28], Dubinin – Radushkevich [29], Temkin [30] isotherms were used for fitting the data (Table 2). Table 2: Two parameter biosorption isotherm models. Model Equation Freundlich qe = KF .Cne qm,L .KL .Ce Langmuir qe = 1 + KL .Ce

linear expression Lnqe = LnKF + n.LnCe 1 1 1 = + qe qm,L .KL .Ce qm,L

976

J. Mater. Environ. Sci. 5 (4) (2014) 975-982 ISSN : 2028-2508 CODEN: JMESCN Dubinin – Radushkevich Temkin

Ainane et al.

-(B.ε2 )

qe = qm,DR .e qe = BT .Ln(KT .Ce )

Lnqe = Lnqm,DR -

R2 T2

E2 qe = BT .LnKT +BT .LnCe

[Ln 1+

1 2 ] Ce

3. Results and discussion 3.1 Kinetic study Studies on the adsorption kinetics of chemical compounds in aqueous solution are usually performed for small ranges of initial concentrations of chemical and adsorbent. The objective was primarily to study the apparent kinetics of adsorption of chromium on four supports that have been already prepared [31]. The kinetic study of biosorption of hexavalent chromium was used to determine the contact time necessary to reach equilibrium. During the contact time, the solution is kept under constant stirring and at constant temperature and pH (pH = 5.8 and T = 25 °C). A mass of 2 g/L of each support and RB crude media activated AB are dispersed in a solution of the chromium to an initial concentration equal to C0 = 50 mg/L. Figure 1 shows the variation of the residual concentration Cres versus time t. 60

Cre s (mg/L)

50 40 RB

30

AB

20 10 0 0

20

40

60 80 100 120 Time (min) Figure 1: Kinetics (residual concentration of chromium Cres vs. time) of Cr(VI) on various forms (RB and AB) of Bifurcaria bifurcata. These curves show two quite clear : A first branch reflects a rapid decrease of the residual concentration of chromium Cres for 20 minutes. A second branch is characterized by a gradual change of the residual concentration of chromium Cres until the balance of biosorption from 60 minutes. The experimental adsorption capacities of activated biomass are higher than those of raw biomass, and the adsorption capacity of the biomass Bifurcaria bifurcata, it increased by 9.42 mg/g to 13.35 mg/g. All the kinetic parameters of biosorption media RB and AB are determined from the straight linearity according to the equations of the models described in Table 1. In considering the reliability of the proposed kinetic models, we calculated the correlation coefficients of the equations and the kinetic constants of each model. These are grouped in Tables 3 and 4. Table 3: Kinetic model parameters for Cr(VI) biosorption on biomasses RB of Bifurcaria bifurcata. Model Fractional power

linear expression y = 0,046x + 2,012

R2 0,886

Elovich

y = 0,409x + 7,391

0,883

pseudo-first order

y = -0,047x + 1,222

0,767

pseudo-second order

y = 0,066x + 0,110

0,577

977

Model parameters υ = 4,6.10-2 kp = 7,478 υ. kp = 0,343 mg.g-1.min-1 αE = 2,863.107 mg.g-1.min-1 βE = 2,444 g.mg-1 k1P = 4,7.10-2 min-1 qe,1P = 3,393 mg.g-1 k2P = 1,666 g.mg-1.min-1 qe,2P = 9,090 mg.g-1

J. Mater. Environ. Sci. 5 (4) (2014) 975-982 ISSN : 2028-2508 CODEN: JMESCN Intraparticle diffusion

Ainane et al.

y = 0,674x + 3,964

0,537

kD = 0,674 mg.g-1.min-1/2 CD = 3,964 mg.g-1

Table 4: Kinetic model parameters for Cr(VI) biosorption on biomasses AB of Bifurcaria bifurcata. Model linear expression R2 Model parameters Fractional power y = 0,031x + 2,440 0,892 υ = 3,1.10-2 ; kp = 11,473 υ. kp = 0,355 mg.g-1.min-1 Elovich y = 0,397x + 11,41 0,890 αE = 1,192.1012 mg.g-1.min-1 βE = 2,518 g.mg-1 pseudo-first order y = -0,056x + 1,388 0,757 k1P = 5,6.10-2 min-1 qe,1P = 4,006 mg.g-1 pseudo-second order y = 0,030x + 0,076 0,597 k2P = 2,533 g.mg-1.min-1 qe,2P = 13,157 mg.g-1 Intraparticle diffusion y = 0,935x + 5,996 0,494 kD = 0,935 mg.g-1.min-1/2 CD = 5,996 mg.g-1

qt (mg;g-1)

From the values of correlation coefficients R2 of these tables we can conclude that the model of fractional power (88.6% to 89.2% for RB and AB) and the Elovich model (88.3% for RB and 89% AB) are closer to the experimental results of adsorption kinetics. By cons, we note that the theoretical data from other models move away from the experimental data. To better demonstrate the effectiveness of the model of fractional power and Elovich model, we reported in Figures 2 and 3 modeling the kinetics of chromium biosorption of these two models respectively on the two biomass RB and AB. 20 18 16 14 RB 12 10 AB 8 Model RB 6 4 Model AB 2 0 0 20 40 Time60(min) 80 100 120

qt (mg;g-1)

Figure 2: Modeling the kinetics of chromium biosorption of the fractional power model. 20 18 16 14 12 10 8 6 4 2 0

RB AB Model RB Model AB

0

20

40

60

80

100

120

Time (min) Figure 3: Modeling the kinetics of chromium biosorption of the Elovich model. 3.2. Equilibrium isotherm models With a view to assess the adsorption capacity of chromium on each support algal prepared a study of adsorption isotherms was carried out. Recall that adsorption isotherm is also known as saturation curve and it shows the variation of the amount adsorbed qt depending on the residual concentration at equilibrium Ce (qt = f (Ce)) at a temperature T and a pH consistent. (T = 25 °C, pH = 5.8) 978

J. Mater. Environ. Sci. 5 (4) (2014) 975-982 ISSN : 2028-2508 CODEN: JMESCN

Ainane et al.

In order to determine the nature of the adsorption isotherm of chromium on the media, we made solutions containing chromium at initial concentrations constant C0 = 50 mg / L, and for each medium we introduced the masses of adsorbent on the volume of the adsorbate of 0.5 g/L to 5 g/L. Stirring is continued for a sufficient time to reach equilibrium (two hours). At the end of each experiment, we determine the residual concentrations of chromium, then we deduce the sorption capacity at equilibrium Qeq. The changes in adsorption capacities at equilibrium according Qeq residual concentrations at equilibrium it is the equilibrium isotherms. Equilibrium isotherms of biosorption of chromium on biomass RB and AB are represented in Figure 4. 30 qeq (mg/g)

25 20

15 10

RB

5

AB

0 0

10

20

30

40

Cres (mg/L) Figure 4: Equilibrium isotherms of biosorption of chromium on biomass RB and AB. To process the experimental data, and to explain the isotherms obtained from equilibrium, we used isothermal models that have been previously described in Table 2. The constants characterizing each of the linear expressions of these models were determined and the data in Table 5 and Table 6 for RB and AB. Note that the reliability of these proposed models was performed by calculating the correlation coefficients R2. Table 5: Isotherms model parameters for Cr(VI) biosorption on RB. Model linear expression

R2

Freundlich

y = 2,294x - 5,585

0,842

Langmuir

y = 7,139x - 0,121

0,947

Dubinin – Radushkevich

y = -971,6x + 3,374

0,776

Temkin

y = 24,87x - 74,00

0,657

Table 6: Isotherms model parameters for Cr(VI) biosorption on AB. Model linear expression

R2

Freundlich

y = 0,856x + 0,116

0,811

Langmuir

y = 0,971x + 0,019

0,821

Dubinin – Radushkevich

y = -121,3x + 3,137

0,64

979

Model parameters n = 2,294 KF = 3,75.10-3 L.g−1 qm,F = 29,641 mg.g-1 n>1 : adsorption faible KL = 1,69.10-2 L.g−1 qm,L = 8,264 mg.g-1 RL = 0,54 B = 1,58.10-4 J2.mol−2 qm,DR = 29,195 mg.g-1 E = 79,446 J.mol−1 BT = 24,87 J.mol−1 KT = 5,1.10-2 L.g−1 ΔQ = 99,57 J qm,T = 23,29 mg.g-1 Model parameters n = 0,856 KF = 1,122 L.g−1 qm,F = 31,966 mg.g-1 0,5

Ainane et al.

Removal of hexavalent chromium from aqueous solution by raw and chemically modified seaweed Bifurcaria bifurcata T. Ainane1,2, A. Abourriche1 , M. Kabbaj2, M. Elkouali2, A. Bennamara1, M. Charrouf1, M. Talbi2 (1) Biomolecules and organic synthesis laboratory, Faculty of Sciences Ben Msik, University Hassan II, BP 7955 casablanca 20660, Morocco. (2) Laboratory of Analytical Chemistry and Physical Chemistry of Materials, Faculty of Sciences Ben Msik, University Hassan II, BP 7955 casablanca 20660, Morocco. Received 11 Nov 2013, Revised 8 May 2014, Accepted 8 May 2014. Email: [email protected] Tel :00 212 (0) 6 60 39 30 90

Abstract The presence of hexavalent chromium Cr(VI) in wastewater is a potential hazard to aquatic animals and humans. There are various mechanisms proposed, kinetic models used and adsorption isotherms employed for the efficient removal of hexavalent chromium from industrial and municipal wastewaters using biosorbents. Biosorption of heavy metals is a most promising technology involved in the removal of toxic metals from industrial waste streams and natural waters. Metal removal treatment systems using natural materialsare cheap because of the low cost of sorbent materials used and may represent a practical replacement to conventional processes. The objective of this study is to assess the uptake of hexavalent chromium from aqueous solutions onto Bifurcaria bifurcata algae raw and chemically modified. The biosorption data of hexavalent chromium by marine brown algae Bifurcaria bifurcata, which was raw RB and chemically modified by hydrochloric acid AB, has been used for kinetic studies based on fractional power, Elovich, pseudo-first order, pseudosecond order and intraparticle diffusion rate expressions. four two parameter biosorption isotherm models, Freundlich, Langmuir, Dubinin – Radushkevich, Temkin are tested for their applicability. The time-dependent Cr(VI) biosorption data were well-described by fractional power and Elovich kinetic model. Among the two-parameter models, the Langmuir model produces the best fit. Comparing our results with other previous work on the brown algae, shows the value of materials developed from Bifurcaria bifurcata and allows us to offer them as adsorbent materials. Keywords: Hexavalent chromium, Bifurcaria bifurcata, Biosorption, Kinetics, Equilibrium models.

1. Introduction The presence of toxic heavy metals in water resulting from rapid industrialization and technological advances is a worldwide environmental problem [1-4]. One of the heavy metals that has been a major focus in water and wastewater treatment is chromium and the hexavalent form of it has been considered to be more hazardous due to its carcinogenic properties [5-7]. Chromium has been considered as one of the top 16th. Toxic pollutants and because of its carcinogenic and teratogenic characteristics on the public, it has become a serious health concern [8]. Chromium can be released to the environment through a large number of industrial operations, including metal finishing industry, iron and steel industries and inorganic chemicals production [9]. Extensive use of chromium results in large quantities of chromium containing effluents which need an exigent treatment. The permissible limit of chromium for drinking water is 0.1 mg/L (as total chromium) in EPA standard (United States Environmental Protection Agency). In addition, World Health Organization standard for Cr(VI) concentration in drinking water is 0.05 mg/L [10-11]. Removal of heavy metals from aqueous effluents has conventionally been accomplished through a range of abiotic processes [12-14]. However, these processes can be expensive and not fully effective. Recently, increasing interest in the application of materials of biological origin in heavy metals removal from diluted, large volume solutions has been observed. Sorption with bio-materials has become an alternative to traditional methods of industrial wastewaters treatment, such as precipitation, adsorption, coagulation, … [15-17] and it is relatively inexpensive, non-hazardous, and may permit recovery of the metals from the sorbing biomass [18]. The potential 975

J. Mater. Environ. Sci. 5 (4) (2014) 975-982 ISSN : 2028-2508 CODEN: JMESCN

Ainane et al.

of nonviable brown seaweeds in the recovery of heavy metal ions from aqueous effluents has been well demonstrated [19,20]. The objective of this study was to evaluate the adsorption capacity of chromium on substrates obtained from the brown seaweed Bifurcaria bifurcata. The choice of the latter is mainly based on purely economic considerations, because we are always looking for natural materials with no obvious utility in order to exploit them for very specific tasks, either in its raw state or after certain operations do not require large investments in energy supply or material. The main objective is to enhance this marine natural resource and use for water-pollution control and preservation of ecological balance.

2. Materials and methods 2.1 Biomass and chemical modification The brown alga Bifurcaria bifurcata was collected from the Dar Bouaaza beach (Casablanca), Morocco in December 2009. The alga was washed with running water and with deionized water. The washed biomass was oven-dried at 60 ◦C for 24 h, crushed with an analytical mill, sieved (size fraction of 0.50 mm). The resulting dried biomass was designated as the raw biomass (RB) in the present study. A 100 g raw biomass was activated in 1M solution of hydrochloric acid at 25 °C for 2h and the mixture was separated by centrifugation and washed thoroughly with distilled water. It was dried in an oven at 60 °C for 24 h. resulting dried biomass was designated as the actived biomass (AB). 2.2 Sorption experiments and analytical method All the experiments were conducted at a constant temperature of 25±1 °C and at a constant pH = 5.8 to be representative of environmentally relevant conditions. Batch kinetics and equilibrium sorption experiments were carried out in 250mL Erlenmeyer flasks containing Potassium dichromate solutions (100 mL) of known concentrations, which varied from 30 to 50 mg L−1. Known amounts of biomass were added to each flask and the mixtures were agitated on the rotary shaker. After the sorption was reached, The change in Cr(VI) concentration due to sorption was determined colorimetrically (Shimadzu 1240 spectrophotometer) according to Standard Methods [21]. A purple-violet colored complex was developed in the reaction between Cr(VI) and 1,5-diphenylcarbazide in acidic condition. Absorbance was measured at wavelength (λ) 540 nm. 2.3 Chromium uptake capacities The amount of Cr(VI) sorbed at equilibrium, q (mg.g−1), which represents the metal uptake, was calculated from the difference in metal concentration in the aqueous phase before and after adsorption, according to the following equation [22] : (C0 -Ce ) q= m C0 and Ce are the initial and equilibrium concentration of Cr(VI) in solution (mg.l−1), respectively, and m is the mass of dry seaweed (g). where V is the volume of Cr(VI) solution (L). Fractional power [23], Elovich [24], pseudo-first order [25], pseudo-second order [24] and intraparticle diffusion [26] rate equations have been used for modeling the kinetics of Cr(VI) sorption (Table 1). Table 1: Kinetic biosorption models. Model Fractional power Elovich pseudo-first order pseudo-second order

Equation qt = kp .tν

1 .Ln(αE .βE .t) βE qt = qe,1P (1-e-k1p .t ) qt =

qt =

k2p .q2e,2P .t

linear expression Ln qt = ν.Ln t + Ln kp Ln(αE .βE ) 1 qt = + .Lnt βE βE Ln qe -qt = -k1p .t + Ln qe,1P 1 1 1 = + qt k2p .qe,2P .t qe,2P

1 + k2p .qe,2P .t Intraparticle diffusion qt = kD .t1/2 + CD To examine the relationship between sorbed and aqueous concentration at equilibrium, various two-parameter sorption isotherm models like Freundlich [27], Langmuir [28], Dubinin – Radushkevich [29], Temkin [30] isotherms were used for fitting the data (Table 2). Table 2: Two parameter biosorption isotherm models. Model Equation Freundlich qe = KF .Cne qm,L .KL .Ce Langmuir qe = 1 + KL .Ce

linear expression Lnqe = LnKF + n.LnCe 1 1 1 = + qe qm,L .KL .Ce qm,L

976

J. Mater. Environ. Sci. 5 (4) (2014) 975-982 ISSN : 2028-2508 CODEN: JMESCN Dubinin – Radushkevich Temkin

Ainane et al.

-(B.ε2 )

qe = qm,DR .e qe = BT .Ln(KT .Ce )

Lnqe = Lnqm,DR -

R2 T2

E2 qe = BT .LnKT +BT .LnCe

[Ln 1+

1 2 ] Ce

3. Results and discussion 3.1 Kinetic study Studies on the adsorption kinetics of chemical compounds in aqueous solution are usually performed for small ranges of initial concentrations of chemical and adsorbent. The objective was primarily to study the apparent kinetics of adsorption of chromium on four supports that have been already prepared [31]. The kinetic study of biosorption of hexavalent chromium was used to determine the contact time necessary to reach equilibrium. During the contact time, the solution is kept under constant stirring and at constant temperature and pH (pH = 5.8 and T = 25 °C). A mass of 2 g/L of each support and RB crude media activated AB are dispersed in a solution of the chromium to an initial concentration equal to C0 = 50 mg/L. Figure 1 shows the variation of the residual concentration Cres versus time t. 60

Cre s (mg/L)

50 40 RB

30

AB

20 10 0 0

20

40

60 80 100 120 Time (min) Figure 1: Kinetics (residual concentration of chromium Cres vs. time) of Cr(VI) on various forms (RB and AB) of Bifurcaria bifurcata. These curves show two quite clear : A first branch reflects a rapid decrease of the residual concentration of chromium Cres for 20 minutes. A second branch is characterized by a gradual change of the residual concentration of chromium Cres until the balance of biosorption from 60 minutes. The experimental adsorption capacities of activated biomass are higher than those of raw biomass, and the adsorption capacity of the biomass Bifurcaria bifurcata, it increased by 9.42 mg/g to 13.35 mg/g. All the kinetic parameters of biosorption media RB and AB are determined from the straight linearity according to the equations of the models described in Table 1. In considering the reliability of the proposed kinetic models, we calculated the correlation coefficients of the equations and the kinetic constants of each model. These are grouped in Tables 3 and 4. Table 3: Kinetic model parameters for Cr(VI) biosorption on biomasses RB of Bifurcaria bifurcata. Model Fractional power

linear expression y = 0,046x + 2,012

R2 0,886

Elovich

y = 0,409x + 7,391

0,883

pseudo-first order

y = -0,047x + 1,222

0,767

pseudo-second order

y = 0,066x + 0,110

0,577

977

Model parameters υ = 4,6.10-2 kp = 7,478 υ. kp = 0,343 mg.g-1.min-1 αE = 2,863.107 mg.g-1.min-1 βE = 2,444 g.mg-1 k1P = 4,7.10-2 min-1 qe,1P = 3,393 mg.g-1 k2P = 1,666 g.mg-1.min-1 qe,2P = 9,090 mg.g-1

J. Mater. Environ. Sci. 5 (4) (2014) 975-982 ISSN : 2028-2508 CODEN: JMESCN Intraparticle diffusion

Ainane et al.

y = 0,674x + 3,964

0,537

kD = 0,674 mg.g-1.min-1/2 CD = 3,964 mg.g-1

Table 4: Kinetic model parameters for Cr(VI) biosorption on biomasses AB of Bifurcaria bifurcata. Model linear expression R2 Model parameters Fractional power y = 0,031x + 2,440 0,892 υ = 3,1.10-2 ; kp = 11,473 υ. kp = 0,355 mg.g-1.min-1 Elovich y = 0,397x + 11,41 0,890 αE = 1,192.1012 mg.g-1.min-1 βE = 2,518 g.mg-1 pseudo-first order y = -0,056x + 1,388 0,757 k1P = 5,6.10-2 min-1 qe,1P = 4,006 mg.g-1 pseudo-second order y = 0,030x + 0,076 0,597 k2P = 2,533 g.mg-1.min-1 qe,2P = 13,157 mg.g-1 Intraparticle diffusion y = 0,935x + 5,996 0,494 kD = 0,935 mg.g-1.min-1/2 CD = 5,996 mg.g-1

qt (mg;g-1)

From the values of correlation coefficients R2 of these tables we can conclude that the model of fractional power (88.6% to 89.2% for RB and AB) and the Elovich model (88.3% for RB and 89% AB) are closer to the experimental results of adsorption kinetics. By cons, we note that the theoretical data from other models move away from the experimental data. To better demonstrate the effectiveness of the model of fractional power and Elovich model, we reported in Figures 2 and 3 modeling the kinetics of chromium biosorption of these two models respectively on the two biomass RB and AB. 20 18 16 14 RB 12 10 AB 8 Model RB 6 4 Model AB 2 0 0 20 40 Time60(min) 80 100 120

qt (mg;g-1)

Figure 2: Modeling the kinetics of chromium biosorption of the fractional power model. 20 18 16 14 12 10 8 6 4 2 0

RB AB Model RB Model AB

0

20

40

60

80

100

120

Time (min) Figure 3: Modeling the kinetics of chromium biosorption of the Elovich model. 3.2. Equilibrium isotherm models With a view to assess the adsorption capacity of chromium on each support algal prepared a study of adsorption isotherms was carried out. Recall that adsorption isotherm is also known as saturation curve and it shows the variation of the amount adsorbed qt depending on the residual concentration at equilibrium Ce (qt = f (Ce)) at a temperature T and a pH consistent. (T = 25 °C, pH = 5.8) 978

J. Mater. Environ. Sci. 5 (4) (2014) 975-982 ISSN : 2028-2508 CODEN: JMESCN

Ainane et al.

In order to determine the nature of the adsorption isotherm of chromium on the media, we made solutions containing chromium at initial concentrations constant C0 = 50 mg / L, and for each medium we introduced the masses of adsorbent on the volume of the adsorbate of 0.5 g/L to 5 g/L. Stirring is continued for a sufficient time to reach equilibrium (two hours). At the end of each experiment, we determine the residual concentrations of chromium, then we deduce the sorption capacity at equilibrium Qeq. The changes in adsorption capacities at equilibrium according Qeq residual concentrations at equilibrium it is the equilibrium isotherms. Equilibrium isotherms of biosorption of chromium on biomass RB and AB are represented in Figure 4. 30 qeq (mg/g)

25 20

15 10

RB

5

AB

0 0

10

20

30

40

Cres (mg/L) Figure 4: Equilibrium isotherms of biosorption of chromium on biomass RB and AB. To process the experimental data, and to explain the isotherms obtained from equilibrium, we used isothermal models that have been previously described in Table 2. The constants characterizing each of the linear expressions of these models were determined and the data in Table 5 and Table 6 for RB and AB. Note that the reliability of these proposed models was performed by calculating the correlation coefficients R2. Table 5: Isotherms model parameters for Cr(VI) biosorption on RB. Model linear expression

R2

Freundlich

y = 2,294x - 5,585

0,842

Langmuir

y = 7,139x - 0,121

0,947

Dubinin – Radushkevich

y = -971,6x + 3,374

0,776

Temkin

y = 24,87x - 74,00

0,657

Table 6: Isotherms model parameters for Cr(VI) biosorption on AB. Model linear expression

R2

Freundlich

y = 0,856x + 0,116

0,811

Langmuir

y = 0,971x + 0,019

0,821

Dubinin – Radushkevich

y = -121,3x + 3,137

0,64

979

Model parameters n = 2,294 KF = 3,75.10-3 L.g−1 qm,F = 29,641 mg.g-1 n>1 : adsorption faible KL = 1,69.10-2 L.g−1 qm,L = 8,264 mg.g-1 RL = 0,54 B = 1,58.10-4 J2.mol−2 qm,DR = 29,195 mg.g-1 E = 79,446 J.mol−1 BT = 24,87 J.mol−1 KT = 5,1.10-2 L.g−1 ΔQ = 99,57 J qm,T = 23,29 mg.g-1 Model parameters n = 0,856 KF = 1,122 L.g−1 qm,F = 31,966 mg.g-1 0,5